# Fluid Transport Phenomena in Fibrous Materials ch3 wetting wicking

```3
LIQUID TRANSPORT IN FIBROUS MATERIALS:
WICKING AND WETTING
3.1 Introduction
Wicking and wetting are among the most frequently observed phenomena in the
processing and use of fibrous materials, when water or any other liquid chemicals comes
into contact with and transport through the fibrous structures. Besides its involvement in
such wetting processes as scouring, dyeing and finishing, wetting and wicking property
of fibrous materials is also a paramount factor in evaluating comfort and performance of
clothing fabrics, hygiene products, etc. Accordingly, extensive research has been carried
out in this field to study the theories, characterization and testing methods, and modeling
and simulation techniques of the wicking and wetting phenomenon.
3.2 Surface tension and interfacial interaction: wicking and wetting theories
3.2.1 Wetting
The term “wetting” is usually used to describe the displacement of a solid-air interface
with a solid-liquid interface. When a small liquid droplet is put in contact with a flat solid
surface, two distinct equilibrium regimes may be found: partial wetting with a finite
contact angle θ, or complete wetting with a zero contact angle [1], as shown in Fig. 1.
Vapor
Liquid
θ
θ
Solid
(a)
(b)
(c)
Fig.1 A small liquid droplet in equilibrium over a horizontal surface:
(a) partial wetting, mostly non wetting, (b) partial wetting, mostly wetting,
(c) complete wetting
The forces in equilibrium at a solid-liquid boundary are commonly described by the
Young’s equation:
 SV   SL   LV cos  0
(3.1)
where γSV, γSL, and γLV denotes interfacial tensions between solid/vapor, solid/liquid and
liquid/vapor, respectively, and θ is the equilibrium contact angle.
The parameter that distinguishes partial wetting and complete wetting is the so called
spreading parameter S, which measures the difference between the surface energy (per
unit area) of the substrate when dry and wet:
1
S  Esubstratedry  Esubstratewet
or
S   SV   SL   LV 
(3.2)
(3.3)
If the parameter S is positive, the liquid spreads completely in order to lower its surface
energy (θ=0). The final outcome is a film of nano-scopic thickness resulting from
competition between molecular and capillary forces.
If the parameter S is negative, the drop does not spread out, but forms at equilibrium a
spherical cap resting on the substrate with a contact angle θ. A liquid is said to be “mostly
wetting” when θ≤π/2, and “mostly non-wetting” when θ&gt;π/2 [2]. When contacted with
water, a surface is usually called “hydrophilic” when θ≤π/2, and “hydrophobic” when
θ&gt;π/2.
3.2.2 Wicking
Wicking is the spontaneous flow of a liquid in a porous substrate, driven by capillary
forces. As capillary forces are caused by wetting, wicking is a result of spontaneous
wetting in a capillary system [3] .
In the simplest case of wicking in a single capillary tube, as shown in Fig.3.2, a meniscus
is formed. The surface tension of the liquid causes a pressure difference across the curved
liquid/vapor interface. The value for the pressure difference of a spherical surface was
deduced in 1805 independently by Thomas Young (1773-1829) and Pierre Simon de
Laplace (1749-1827), and is represented with the so called Young-Laplace equation [4]:
 1
1 

(3.4)
P   LV  
R
R
2 
 1
For a capillary with a circular cross section, the radii of the curved interface R1 and R2 are
equal. Thus:
P  2 LV R
(3.5)
where
(3.6)
R  r cos 
and r is the capillary radius. As the capillary spaces in a fibrous assembly are not uniform,
usually an indirectly determined parameter, effective capillary radius re is used instead.
r
R
θ
h
Fig.3.2 Wicking in a capillary
2
3.2.3 Surface tension and interfacial interactions
The above discussions show that both wicking and wetting behaviors are determined by
surface tensions (of solid and liquid) and liquid/solid interfacial tensions. These
surface/interfacial tensions, in macroscopic concepts, can be defined as the energy that
must be supplied to increase the surface/interface area by one unit. In microscopic
concepts, however, they are originated from such intra-molecular bounds as covalent,
ionic or metallic, and such long range intermolecular forces as van der Waals forces.
Therefore, the physical basis of wetting and wicking are those molecular interactions
within a solid or liquid, or across the interface between liquid and solid.
Macroscopic: Wettability
From studies on the bulk cohesive energy, we learn that there are two main types of
solids: hard solids (bound by covalent, ionic or metallic) with the so called “high energy
surfaces”, and weak molecular crystals (bound by van der Waals forces, or in some
special cases by hydrogen bond) with “low energy surfaces”. The surface tension, γsv, is
in the range of 500 to 5,000mN/m for high energy surfaces, and 10 to 50mN/m for low
energy surfaces [5]. Most organic fibers belong to the “low energy surfaces” category.
Most molecular liquids achieve complete wetting with high-energy surfaces [1]. In the
idealized case where liquid/liquid and liquid/solid interactions are purely of the van der
Waals type (no chemical bonding), solid/liquid energy could be deducted as follows:
If a semi-infinite solid and a semi-infinite liquid are brought together, they start with an
energy γLV+ γSV, and end in γSL, as the van der Waals interaction energy VSL between solid
and liquid VSL is consumed. This process can be expressed as:
 SL   SV   LV  VSL
(3.7)
To a first approximation the van der Waals couplings between two species are simply
proportional to the product of the corresponding polarizabilities α [1]:
(3.8)
VSL  k S  L
Similarly, if two liquid portions are brought together, they start with energy 2γLV, and end
up with zero interfacial energy:
2 LV  VLL  0
(3.9)
The same applies to solid:
2 SV  VSS  0
(3.10)
Equation (3.3) combined with (3.7)-(3.10) gives:
S   SV   SL   LV   VSL  VLL  k  S   L  L
(3.11)
Therefore, a liquid spreads completely if αS&gt;αL so as to make S positive.
Low-energy surfaces can give rise to partial or complete wetting, depending on the liquid
chosen [1]. The empirical criterion of Zisman [2, 6] is that each solid substrate has a
critical surface tension γC, and there is partial wetting when the liquid surface tension
γ&gt;γC and total wetting when γ&lt;γC.
3
The critical surface tension can be determined by the so called Zisman plot. A series of
homologous liquid (usually n-alkanes, with n the variable) is chosen for the study. Cosθ
as a function of γ is plotted to give the critical surface tension, as shown in Fig.3.3.
Critical surface tension of some solid polymers is shown in Table 3.1 [1, 2].
cosθ
1
0
γC
γ
o
f
n-alkanes(mN/m)
Fig.3.3 A typical Zisman plot to determine critical surface tension γC
Table 3.1 Critical surface tension γC of several solid polymers
Solid
Nylon
PVC
PE
PVF2
γC (mN/m)
46
39
31
28
PVF4
18
Microscopic: Van der Waals forces:
Molecules can attract each other at moderate distances and repel each other at close range,
as denoted by Lennard-Jones potential:
A C
wr   12  6
(3.12)
r
r
where w(r) is the interactive potential between two molecules at distance r, and A and C
are the intensities of the repellency and attraction, respectively.
The attractive forces, represented by the second term at the right hand side of equation
(3.12), are collectively called &quot;van der Waals forces&quot;. It is one of the most important
long-range forces between macroscopic particles and surfaces. Van der Waals forces are
much weaker than chemical bonds, and random thermal agitation, even around room
temperature, can usually overcome or disrupt them. However, they play a central role in
all phenomena involving intermolecular forces, including those actions between
electrically neutral molecules [7].
When those intermolecular forces are between like molecules, they are referred to as
cohesive forces. For example, the molecules of a water droplet are held together by
cohesive forces. The cohesive forces between molecules inside a liquid are shared with
all neighboring atoms. Those on the surface have no neighboring atoms beyond the
surface, and exhibit stronger attractive forces upon their nearest neighbors on the surface.
4
This enhancement of the intermolecular attractive forces at the surface is called surface
tension, as shown in Fig.3.4.
Surface Tension
Gas
Liquid
Fig.3.4 Liquid surface tension caused by cohesive forces between liquid molecules
Intermolecular forces between different molecules are known as adhesive forces. They
are responsible for wetting and capillary phenomena. For example, if the adhesive forces
between a liquid and a glass tube inner surface are larger than the cohesive forces within
the liquid, the liquid will rise upwards along the glass tube to show capillary phenomenon,
as shown in Fig.3.2.
To derive the van der Waals interaction energy between two bodies/surfaces from the
pair potential wr    C r 6 , Hamaker [8] introduced an additivity assumption that the
total interaction can be seen as the sum over all pair interactions between any atom in one
body and any atom in the other, thus obtaining the “two body” interaction energy, such as
that for two spheres (Fig.3.5 (a)), for a sphere near a surface (Fig.3.5(b)), and for two flat
surfaces (Fig.3.5(c)) [7]. And the Hamaker constant A is given as a function of densities
of the two bodies:
(3.13)
A   2C1 2
D
R1
ρ1
R2
ρ2
(a) Two Spheres
A R1 R2
W 
6 D R1  R2
R
D
(b) Sphere-Surface
AR
W 
6D
D
(c) Two Surfaces
A
W 
12D 2
per unit area
Fig.3.5 Van der Waals interaction free energies between selected bodies.
Hamaker’s theory has ever since been used widely in studies of surface/interface
interactions and wetting phenomena, although there have been concerns about its
5
additivity assumption and ignorance of the influence of neighboring atoms on the
interaction between any atom pairs [7, 9].
The problem of additivity is completely avoided in Lifshitz’s theory [7, 9-11]. The
atomic structure is ignored, and interactive bodies are regarded as dielectric continuous
media. Then the forces between large bodies can be derived in terms of such bulk
properties as their dielectric constants and refractive indices. And the net result of a rather
complicated calculation is that Lifshitz regained the Hamaker expressions in Fig. 3.5, but
with a different interpretation of the Hamaker constant A. An approximate expression for
the Hamaker constant of two bodies (1 and 2) interacting across a medium 3, none of
them being a conductor, is [7, 9]
A1, 2 

 n  n 
2 n  n  n  n  n  n   n
3hve n12  n32
8
2
1
2 1/ 2
3
2
2
2 1/ 2
3
2
2
2
1
2
3
2 1/ 2
3
2
2

2 1/ 2
3
n

3      3
 kT 1 3 2
4 1   3  2   3
(3.14)
where h is the Planck’s constant, ve is the main electronic adsorption frequency in the UV
(assumed to be the same: for the three bodies, and typically around 31015 s-1), and ni is
the refractive index of phase i, i is the static dielectric constant of phase i, k is the
Boltzmann constant, and T the absolute temperature.
3.3 Liquid Penetration through fibrous materials
There has been numerous research work published on wetting process on solid surface,
including several comprehensive reviews [1, 12], which cover topics from contact angle,
contact line, liquid/solid adhesion, to wetting transition (from partial wetting to complete
However, wetting of fibrous materials becomes an even more complex process due to at
least two factors:
i)
There is the interaction of liquid with a porous medium of intricate,
tortuous and yet soft surface, instead of a simple solid one.
ii)
There are often imbibitions of liquid into the interior of the fibers, which
may cause changes in the structure and properties of the fibrous materials.
3.3.1 Wicking Dynamics
Most textile processes are time limited, so the kinetics of wicking becomes very
important. The classical Washburn-Lucas equation [13] describes the liquid’s velocity,
dh/dt, moving up or down in a perpendicular capillary with the radius r, neglecting the
inertia of the liquid column.
dh r cos
(3.15)

dt
4h
where η is the viscosity of liquid, γ the surface tension and ρ the density of liquid.
6
To apply the Washburn equation into wicking studies, Minor [14, 15] used several kinds
of liquid in his wicking experiments and established that the wicking height of liquid in a
fiber or yarn was proportional to the square root of the time
1
 r cos   2
h  Wct  
t 
(3.16)
 2

According to Equation (3.16), the height of the liquid front will keep rising with time.
Actually, however, the liquid column will cease to rise after a certain period of time due
to the balance of surface tension and gravity. And, the parameter r is hard to determine as
the yarn is not geometrically equivalent to a capillary tube. Furthermore, the equation
incorrectly assumes a constant advancing contact angle for the moving liquid front.
Despite of these limitations, a variety of liquids were still reported to obey the Washburn
kinetics [16].
1
2
Also, a lot of works has been dedicated to the modification of the Washburn equation. In
some early work, constants or coefficients were adopted to account for the difference
between wicking theories and experiments, such as a hydraulic constant [17], which
representing the porous structure of fibrous materials.
Other work trying to accommodate the effect of gravity [18-21]. The Washburn equation
that includes the effect of gravity contains two constants:
(3.17)
At  Bt  ln 1  Bt 
where g is the gravitational constant and
 2 g 2r 3
gr
(3.18)
A
,
B
16 cos 
2 cos 
Equation (3.17) is not analytically solvable, and usually requires approximation or
experimental fit. Recently, some researchers have been trying to incorporate the gravity
effect into the wicking process by means of statistical mechanics (i.e., modeling and
simulation [22-26]. Details of these modeling and simulation techniques will be discussed
in section 3.5.
In addition, dynamic contact angle has been discussed in the studies of wicking dynamics.
It can be given either with an empirical equation [19, 27] or experimental analysis [2830]. Quere and Di Meglio [27] showed that, in a capillary rise of silicone oil along a
vertical thin fiber, most of the rising time is spent in a long regime of relaxation towards
equilibrium, where θ varies to t-1/2. Clanet and Quere [30] experimentally studied the
dynamical phenomenon of capillary rise in a vertical fiber with liquids of low and high
viscosity, and also found the dynamic angle θ scales to t-1/2. More recently, various
modeling methods, such as molecular kinetics, molecular hydrodynamics [31], and
molecular dynamics [32-34] has been used to study the dynamic evolution of contact
angle during the wicking process. And Seveno [32] predicts that there are two different
time scale behaviors within the wicking process related to the two dissipation channels:
friction between the liquid and the solid, leading to t-1, and hydrodynamics, leading to t-1/2.
7
Wicking is also affected by the morphology of fibrous assemblies. Most fibrous
structures are never of a perfect capillary, and are changeable due to swelling of fibers (if
hydrophilic) [35, 36], and can therefore further complicate the problem [37]. Although
there have been reported studies on deriving equivalent capillary radius and equivalent
contact angles for wicking problems in fibrous materials [38], as well as wicking flow on
periodically irregular capillaries [39], an efficient and precise way of representing the
intricate structure of fibrous structures is still demanding.
3.3.2 Wetting and wetting dynamics
Wetting of fibrous materials is dramatically different from wetting process on a flat
surface due to the geometry of the cylindrical shape. A liquid that fully wets a material in
the form of a smooth planar surface may not wet the same material when presented as a
smooth fiber surface.
Brochard [40] discussed the spreading of liquids on thin cylinders, and stated that, for
nonvolatile liquids, a liquid drop cannot spread out over the cylinder if the spreading
coefficient S is smaller than a critical value Sc, instead of 0. At the critical value Sc, there
is a first order transition from a droplet to a sheath structure (“manchon”). The critical
value was derived as
2
3 a 3
Sc    
2 b
where a is the molecular size, b is the radius of the cylinder.
(3.19)
There was also plenty of research work on the equilibrium shapes of liquid drops on
fibers [41-50]. It was reported that two distinctly different geometric shapes of droplet are
possible: a barrel and a clam shell, as shown in Fig.3.6.
x1
x2
Fiber
(a) Barrel Shape
(b) Clam-shell shape
Fig.3.6 Equilibrium Liquid Droplet Shapes on a Fiber
In the absence of gravity, the equilibrium shape of a drop surface is that the Laplace
excess pressure, as shown in Equation (3.4), across the drop surface is everywhere
constant. Carroll [47] solved this equation for the axially symmetric barrel shape subject
to the boundary condition that the profile of the fluid surface meets the solid at an angle
given by the equilibrium contact angle θ:
8
2 LV n  cos  
x1 n 2  1
where n=x2/x1, is the reduced radius as shown in Fig.3.6(a).
P 


(3.20)
Carroll’s solution for the barrel shape droplet was subsequently used to compute the
surface free energy, defined as [42]:
(3.21)
F   LV ALV   SL   SV ASL
where ALV and ASV are the liquid/vapor and solid/liquid interfacial areas, respectively.
In contrast to the barrel shape droplet problem, no solution to Laplace’s equation for the
asymmetric clam-shell shape is reported except for such numerical approaches as finite
element methods [50]. There were, however, literatures discussing the roll-up (barrel to
clam-shell) transition [50, 51] in the wetting process on a fiber.
In addition, there was work with respect to gravitational distortion of Barrel-shape
droplets on vertical fibers [52]. To represent the heterogeneous nature of fibrous
materials in the wetting process, Mullins et. al. [53] incorporated a microscopic study of
the effect of fiber orientation on the fiber wetting process when subjected to gravity,
trying to account for the asymmetry of wetting behavior due to fiber orientation and
gravity. The theory concerning the droplet motion and flow on fibers is based on the
balance between drag force, gravitational force and the change in surface tension induced
by the change in droplet profile as the fiber is angled. As a result, there comes out an
angle where droplet flow will be maximized.
In reality, fibrous materials are porous media with intricate, tortuous and yet soft surface,
further complicating the situation. As a result, a precise description of the structure of a
fibrous material can be tedious. Therefore, much research work adopted Darcy’s law, an
empirical formula that describes laminar and steady flow through a porous medium in
terms of the pressure gradient and the intrinsic permeability of the medium [54-56]:
K
(3.22)
u   p

where u is the average velocity of liquid permeation into fibrous materials, μ the
Newtonian viscosity of the liquid, K the permeability, and p the pressure gradient. In
the case of wetting, the driving pressure is usually the capillary pressure as calculated by
the Laplace equation. The permeability K is either determined by experiments or the
empirical Kozeny-Carman relations as a function of fiber volume fraction [56].
This approach, as adopted dominantly in solving problems of resin flow through fibrous
preforms during composite fabrication, will be discussed in greater details in the next
chapter. Darcy’s law reflects the relationship of pressure gradient and average velocity
only in a macroscopic scale, and it can not reach the microscopic details of the liquid
penetration in fibrous media. Accordingly, many researchers trying to solve these
problems by various modeling and simulation techniques, which will be discussed in
details in section 3.5.
9
3.4 Characterization techniques for wicking and wetting behavior of fibrous
materials
Incorporated with various theories for wicking and wetting behaviors of fibrous materials,
a series of characterization techniques have been developed to measure such important
parameters as interfacial tension/energy, contact angle, liquid transport rate (either in
volume or weight) or the liquid profile of fibrous materials. These techniques provide
information for better understanding wicking/wetting behaviors of fibrous materials as
well as for validation of the wicking/wetting theories.
3.4.1 Measuring liquid/fiber contact angle
The most common method of measuring the contact angle is to observe a sessile drop
with a telescope or microscope, as shown in Fig. 3.7. The contact angle is either
determined directly with a goniometer, or the image is recorded by a video system and
the contour is fitted by a computer using the Laplace equation. For small drops where
hydrostatic effects are negligible, the contact angle can be calculated from the height of
the drop h and contact radius a[57]:
  h
tan   
(3.23)
2 a
Alternatively, the contact angle can be measured at the edge of a bubble, as shown in Fig.
3.7 (b). A bubble is positioned usually at the top of a cell which is otherwise filled with
liquid. This method is less sensitive to interface pollution [58].
Solid
θ
h
θ
Gas
a
R
Solid
(a) Sessile drop
Liquid
(b) Sessile bubble
Fig.3.7 Sessile drop and sessile bubble on a planar surface for measuring contact angle.
The above methods can be used to measure the contact angle of a liquid on a planar
fabric, but is difficult if possible to deal with contact angle of a liquid on a filament due
to the steep change in drop profile near the drop edge.
Bascom [59] avoided this problem by suspending a relatively large drop of liquid in a slit
platinum loop as shown in Fig. 3.8. The fiber is secured on a micro-positioner so that the
fiber can be precisely moved through a slit in the loop into the center of the drop, where
the surface is relatively flat, thus avoiding the curvature problem of a single droplet. The
fiber can be moved in vertical direction so that both receding and advancing angles can
10
be observed. This technique could easily resolve contact angles of 40&deg; or higher, but
optical interference problems near the drop edge were encountered for lower angles.
Single Filament
Slit
Plantinum Loop
Liquid drop
Fig.3.8 Single filament contact angle measurement.
More recently, measurement of contact angles on a single fiber was more frequently
carried out by extracting droplet-on-fiber profile using various digital image processing
techniques [60-63], or using such advanced techniques as ESEM (environmental
scanning electron microscope) [64, 65] to improve the reliability and accuracy of results
obtained. The geometry of the extracted droplet-on-fiber profile provides diverse
characteristic drop parameters for the calculation of contact angles, including maximum
drop length and height, drop volume, contact areas, inflection angle, etc. Various
methods are available based on different combination of these parameters [43, 66].
3.4.2 Measuring fiber/liquid interfacial tension/energy
The most sensitive and widely used methods of measuring the wettability of single
filaments is to measure the interfacial adhesion tension by using a recording electromicrobalance, or the “Wilhelm method” [59, 67-69], as shown in Fig. 3.9. The fiber is
suspended from one arm of an electro-balance and is partially submerged in a beaker of
the test liquid. The platform holding the test liquid is mechanically moved in the vertical
direction so that the advancing and receding angles can be measured.
Micro-balance
Fiber
Wetting liquid
Mechanical platform
Fig.3.9 The Wilhelm method for measuring interfacial tension between liquid/fiber
11
The total force on the fiber is
FT  2r LV cos    L gr 2 h
(3.24)
where r is the fiber radius, h the depth of the fiber immersion and g the gravitational
constant.
The first term on the RHS of Equation (3.24) represents the adhesion tension of the liquid
on the fiber. The second term is the buoyant weight of the submerged fiber segment.
Weight of the rest fiber (not submerged), and its support system, is tared off before the
wetting test starts.
Also, the buoyancy term is negligible for thin fibers (r&lt;50μm). Consequently, for thin
fibers the measured force is independent of fiber depth:
(3.25)
FT  2r LV cos 
The contact angle can then be calculated as
mg
cos  
(3.26)
d LV
where m is the balance output. This is also an indirect way of determining the contact
angle. Results obtained with this method often lack reproducibility [70], however.
3.4.3 Measuring liquid transport rate or profile in fibrous materials
Harnett et al. published a comprehensive review on the laboratory test methods for
measuring wicking. They include strip test, plate test, spot test, and siphon test [71].
Among these the most frequently used is the strip test [72-75]. A strip of test fabric (or a
single filament/yarn) is suspended vertically with its lower end immersed in a reservoir of
liquid, to which a dye may be added for tracking the movement of the liquid. The height
reached by the liquid in the fabric (filament/yarn) above the liquid surface level in the
reservoir is measured either after a certain period of time, or recorded continuously by
some image analysis/data collecting apparatus.
In addition to the above direct visualization test methods, indirect measuring methods
were also used to assess the wicking behaviors of fibrous materials, such as the electrical
capacity/resistance techniques [76, 77]. With these, rise of the liquid water in the yarn
trigger an electrical circuit that can be coupled with a personal computer, so that the
distance of water rise as a function of time can be determined.
3.5 Computer experiments: simulation techniques for liquid transport in fibrous
materials
The above sections have already been dealing with theories and experimental testing
techniques for liquid transport in fibrous materials. In a typical experiment, the system is
subjected to measurements, and results, expressed in numeric form, are obtained. Now in
theory, a model of the system can be constructed, usually in the form of a set of
12
mathematical equations, and can then be validated by its ability to describe the system
behavior in certain selected cases; however, this generally implies a considerable amount
of simplification in order to eliminate some of the complexities associated with real
world problems, and to make the problem mathematically tractable.
To be specific, the simplifications involved in many liquid transport models include
substituting the intricate and tortuous fibrous structure with an average parameter such as
porosity, solidity or permeability. This will give rise to error during calculation and
prediction of transport behavior of liquid in fibrous materials, especially those in the
micro/nano scale materials. Accordingly, various computer simulation techniques have
been applied in this field to accommodate more complexity so as to investigate more
realistic systems, and to better understand and explain experiment results. These
techniques are also known as computer experiments.
Molecular Dynamics (MD) and Monte Carlo (MC) are best-known, standard simulation
formulas emerging from the last decades [78] and, accordingly, most of the simulation
for clarifying liquid wetting and transport behaviors falls into these two categories.
Fundamentally, wetting and transport behaviors of liquid in fibrous materials stem from
interactions between liquid/solid and within liquid at the microscopic level. The most
important task for the various models and simulations is, therefore, to define and treat
these interactions.
In Molecular Dynamics, all potentials between atoms, solid as well as liquid, are
described with the standard pairwise Lennard-Jones interactions:
   ij 12   ij 6 
(3.27)
Vij r   4 ij       
 r 
r  



where r is the distance between any pair of atoms i and j, εij is an energy scale (actually
the minimum of the potential), and σij is a length scale (the distance at which the potential
diminishes to zero).
Large scale MD simulations have been adopted to study the spreading of liquid drops on
top of flat solid substrate [33, 34, 79]. If the system contains enough liquid molecules, the
macroscopic parameters, such as the density, surface tension, viscosity, flow patterns and
dynamic contact angle, can be “measured” in the simulation.
However, the computational cost for MD simulations is huge, as they are dealing with the
individual behaviors of a great amount of single molecules. Also, the application of MD
simulations for liquid spreading on a fiber or transport in intricate fibrous structures is
still pending.
To solve the problem of huge computation, simulation techniques have been invented to
cope with the so called “cell”, or small unit of the system, instead of single molecules.
The statistical genesis of the process of liquid penetration in fibrous media can be
regarded as the interactions and the resulting balance among the media and liquid cells
13
that comprise the ensemble. This process is driven by the difference of internal energy of
the system after and before a liquid move from one cell to the other.
In 1990s. Manna et al. [80] presented a 2D stochastic simulation of the shape of a liquid
drop on a wall due to gravity. The simulation was based on the so called Ising’s model
and Kawasaki dynamics. Lukkarinen [81] studied the mechanisms of fluid droplet
spreading on flat solids using a similar model. However, their studies dealt only with
flow problems in a flat surface instead of a real heterogeneous structure. Only recently is
the Ising’s model used in the simulation of wetting dynamics in heterogeneous fibrous
structures [22-26].
As a “meso-scale” approach, stochastic models and simulations deal with discrete and
digitalized cells or subsystems instead of individual molecules. They lead to considerable
reduction of computational cost, naturally.
Detailed information about these simulation techniques will be discussed in Chapter 8,
dedicated to multi-scale approaches, which represent examples of micro- and meso-scale
methods in the study of liquid transport phenomena in fibrous materials.
3.6 Summary
Wicking and/or wetting are among the most frequently encountered phenomena when
processing and using fibrous materials. Wetting is a process of displacing a solid-air
interface with a solid-liquid interface, while wicking is a result of spontaneous wetting in
a capillary system.
The subject of wetting and capillary wicking has been a complex topic attracting
extensive research interests in both theoretical and experimental physics. The special
structure of fibrous materials further complicate the problem of liquid transport behaviors
in porous media of intricate, tortuous and yet soft structure, which may subject to change
due to imbibitions.
In this chapter, recent advances in studying wetting and wicking behaviors on a single
fiber/filament as well as through fibrous assemblies are reviewed. In addition to wetting
theories and the various testing techniques, a couple of computer simulation methods are
briefly mentioned. Further, more intensive research work is demanded, of course, before
a comprehensive understanding of the behaviors of liquid wetting/wicking in fibrous
14
References
1.
2.
3.
4.
5.
6.
7.
8.
9.
10.
11.
12.
13.
14.
15.
16.
17.
18.
19.
20.
de Gennes, P.G., Wetting - Statics and Dynamics. Reviews of Modern Physics,
1985. 57(3): p. 827-863.
de Gennes, P.-G., F. Brochard-Wyart, and D. Quere, Capillarity and wetting
phenomena : drops, bubbles, pearls, waves. 2004, New York: Springer. xv, 291.
Kissa, E., Wetting and wicking. Textile Research Journal, 1996. 66(10): p. 660668.
Adamson, A.W. and A.P. Gast, Physical chemistry of surfaces. 6th ed. 1997, New
York: Wiley. xxi, 784.
Fowkes, F.M., W.A. Zisman, and American Chemical Society. Division of
Colloid and Surface Chemistry., Contact angle, wettability and adhesion; the
Kendall award symposium honoring William A. Zisman, Los Angeles, Calif., April
2-3, 1963. 1964, Washington,: American Chemical Society. ix, 389.
Series, F.M. Fowkes, Editor. 1964: Washingdon, D. C.
Israelachvili, J.N., Intermolecular and surface forces. 2nd ed. 1991, London ; San
Diego, CA: Academic Press. xxi, 450.
Hamaker, H.C., The London van der Waals attraction between spherical particles.
Physica, 1937. 4(10): p. 1058-1072.
Wennerstrom, H., The van der Waals interaction between colloidal particles and
its molecular interpretation. Colloids and Surfaces a-Physicochemical and
Engineering Aspects, 2003. 228(1-3): p. 189-195.
Garbassi, F., M. Morra, and E. Occhiello, Polymer surfaces : from physics to
technology. Rev. and updated ed. 1998, Chichester, England ; New York: Wiley.
ix, 486.
Wu, S., Polymer interface and adhesion. 1982, New York: M. Dekker. xiii, 630.
Good, R.J., Contact-Angle, Wetting, and Adhesion - a Critical-Review. Journal of
Adhesion Science and Technology, 1992. 6(12): p. 1269-1302.
Washburn, E.W., The dynamics of capillary flow. Physical Review, 1921. 17: p.
273-283.
Minor, F.W., The migration of liquids in textile assemblies, Part II. Textile
Research Journal, 1959. 29: p. 931.
Minor, F., W., The migration of liquids in textile assemblies, part III. Textile
Research Journal, 1959. 29: p. 941.
Hodgson, K.T. and J.C. Berg, The Effect of Surfactants on Wicking Flow in Fiber
Networks. Journal of Colloid and Interface Science, 1988. 121(1): p. 22-31.
Chwastiak, S., A Wicking method for measuring wetting propertiws of carbon
yarns. Journal of Colloid and Interface Science, 1973. 42(2): p. 298-309.
Good, R.J. and N.J. Lin, Rate of Penetration of a Fluid into a Porous Body .2.
Verification of Generalization of Washburn Equation, for Organic Liquids in
Glass Capillaries. Journal of Colloid and Interface Science, 1976. 54(1): p. 52-58.
Joos, P., P. Vanremoortere, and M. Bracke, The Kinetics of Wetting in a Capillary.
Journal of Colloid and Interface Science, 1990. 136(1): p. 189-197.
Marmur, A., Penetration and Displacement in Capillary Systems of Limited Size.
Advances in Colloid and Interface Science, 1992. 39: p. 13-33.
15
21.
22.
23.
24.
25.
26.
27.
28.
29.
30.
31.
32.
33.
34.
35.
36.
37.
38.
39.
40.
Marmur, A. and R.D. Cohen, Characterization of porous media by the kinetics of
liquid penetration: The vertical capillaries model. Journal of Colloid and
Interface Science, 1997. 189(2): p. 299-304.
Lukas, D., E. Glazyrina, and N. Pan, Computer simulation of liquid wetting
dynamics in fiber structures using the Ising model. Journal of the Textile Institute,
1997. 88(2): p. 149-161.
Lukas, D. and N. Pan, Wetting of a fiber bundle in fibrous structures. Polymer
Composites, 2003. 24(3): p. 314-322.
Zhong, W., X. Ding, and Z.L. Tang, Modeling and analyzing liquid wetting in
fibrous assemblies. Textile Research Journal, 2001. 71(9): p. 762-766.
Zhong, W., X. Ding, and Z.L. Tang, Statistical modeling of liquid wetting in
fibrous assemblies. Acta Physico-Chimica Sinica, 2001. 17(8): p. 682-686.
Zhong, W., X. Ding, and Z.L. Tang, Analysis of fluid flow through fibrous
structures. Textile Research Journal, 2002. 72(9): p. 751-755.
Quere, D. and J.M. Di Meglio, The Meniscus on a Fiber. Advances in Colloid and
Interface Science, 1994. 48: p. 141-150.
Chibowski, E. and F. Gonzalezcaballero, Theory and Practice of Thin-Layer
Wicking. Langmuir, 1993. 9(1): p. 330-340.
Sauer, B.B. and T.E. Carney, Dynamic Contact-Angle Measurements on GlassFibers - Influence of Fiber Diameter on Hysteresis and Contact Line Pinning.
Langmuir, 1990. 6(5): p. 1002-1007.
Clanet, C. and D. Quere, Onset of menisci. Journal of Fluid Mechanics, 2002. 460:
p. 131-149.
Schneemilch, M., et al., Dynamic wetting and dewetting of a low-energy surface
by pure liquids. Langmuir, 1998. 14(24): p. 7047-7051.
Seveno, D. and J. De Coninck, Possibility of different time scales in the capillary
rise around a fiber. Langmuir, 2004. 20(3): p. 737-742.
Blake, T.D., et al., Contact angle relaxation during droplet spreading:
Comparison between molecular kinetic theory and molecular dynamics.
Langmuir, 1997. 13(7): p. 2164-2166.
de Ruijter, M.J., T.D. Blake, and J. De Coninck, Dynamic wetting studied by
molecular modeling simulations of droplet spreading. Langmuir, 1999. 15(22): p.
7836-7847.
Nederveen, C.J., Absorption of Liquid in Highly Porous Nonwovens. Tappi
Journal, 1994. 77(12): p. 174-180.
Ibbett, R.N. and Y.L. Hsieh, Effect of fiber swelling on the structure of lyocell
fabrics. Textile Research Journal, 2001. 71(2): p. 164-173.
Schuchardt, D.R. and J.C. Berg, Liquid Transport in Composite CelluloseSuperabsorbent Fiber Networks. Wood and Fiber Science, 1991. 23(3): p. 342357.
Marmur, A., Kinetics of penetration into uniform porous media: Testing the
equivalent-capillary concept. Langmuir, 2003. 19(14): p. 5956-5959.
Staples, T.L. and D.G. Shaffer, Wicking flow in irregular capillaries. Colloids and
Surfaces a-Physicochemical and Engineering Aspects, 2002. 204(1-3): p. 239-250.
Brochard, F., Spreading of Liquid-Drops on Thin Cylinders - the ManchonDroplet Transition. Journal of Chemical Physics, 1986. 84(8): p. 4664-4672.
16
41.
42.
43.
44.
45.
46.
47.
48.
49.
50.
51.
52.
53.
54.
55.
56.
57.
58.
Neimark, A.V., Thermodynamic equilibrium and stability of liquid films and
droplets on fibers. Journal of Adhesion Science and Technology, 1999. 13(10): p.
1137-1154.
McHale, G., et al., Estimation of contact angles on fibers. Journal of Adhesion
Science and Technology, 1999. 13(12): p. 1457-1469.
McHale, G., et al., Wetting of a high-energy fiber surface. Journal of Colloid and
Interface Science, 1997. 186(2): p. 453-461.
Quere, D., Fluid coating on a fiber. Annual Review of Fluid Mechanics, 1999. 31:
p. 347-384.
Bauer, C., T. Bieker, and S. Dietrich, Wetting-induced effective interaction
potential between spherical particles. Physical Review E, 2000. 62(4): p. 53245338.
Bieker, T. and S. Dietrich, Wetting of curved surfaces (vol 252, pg 85, 1998).
Physica A, 1998. 259(3-4): p. 466-467.
Carroll, B.J., Accurate Measurement of Contact-Angle, Phase Contact Areas,
Drop Volume, and Laplace Excess Pressure in Drop-on-Fiber Systems. Journal of
Colloid and Interface Science, 1976. 57(3): p. 488-495.
Carroll, B.J., The Equilibrium of Liquid-Drops on Smooth and Rough CircularCylinders. Journal of Colloid and Interface Science, 1984. 97(1): p. 195-200.
Carroll, B.J., Direct Measurement of the Contact-Angle on Plates and on Thin
Fibers - Some Theoretical Aspects. Journal of Adhesion Science and Technology,
1992. 6(9): p. 983-994.
McHale, G. and M.I. Newton, Global geometry and the equilibrium shapes of
liquid drops on fibers. Colloids and Surfaces a-Physicochemical and Engineering
Aspects, 2002. 206(1-3): p. 79-86.
Carroll, B.J., Equilibrium Conformations of Liquid-Drops on Thin Cylinders
under Forces of Capillarity - a Theory for the Roll-up Process. Langmuir, 1986.
2(2): p. 248-250.
Kumar, A. and S. Hartland, Measurement of Contact Angles from the Shape of a
Drop on a Vertical Fiber. Journal of Colloid and Interface Science, 1990. 136(2):
p. 455-469.
Mullins, B.J., et al., Effect of fiber orientation on fiber wetting processes. Journal
of Colloid and Interface Science, 2004. 269(2): p. 449-458.
Yoshikawa, S., et al., Experimental-Study of Flow Mechanics in a Hollow-Fiber
Membrane Module for Plasma Separation. Journal of Chemical Engineering of
Japan, 1992. 25(5): p. 515-521.
Ghali, K., B. Jones, and J. Tracy, Experimental-Techniques for Measuring
Parameters Describing Wetting and Wicking in Fabrics. Textile Research Journal,
1994. 64(2): p. 106-111.
Mao, N. and S.J. Russell, Anisotropic liquid absorption in homogeneous twodimensional nonwoven structures. Journal of Applied Physics, 2003. 94(6): p.
4135-4138.
Dimitrov, A.S., et al., Contact-Angle Measurements with Sessile Drops and
Bubbles. Journal of Colloid and Interface Science, 1991. 145(1): p. 279-282.
Butt, H.-J., K. Graf, and M. Kappl, Physics and chemistry of interfaces. 2003,
Weinheim: Wiley-VCH. xii, 361.
17
59.
60.
61.
62.
63.
64.
65.
66.
67.
68.
69.
70.
71.
72.
73.
74.
75.
Bascom, W.D., The wetting behavior of fibers, in Modern Approaches to
Wettability: Theory and Applications, Malcolm E. Schrader and G. Loeb, Editors.
1992, Plenum Press: New York. p. 359-373.
Lee, Y.N. and S.M. Chiao, Visualization of dynamic contact angles on cylinder
and fiber. Journal of Colloid and Interface Science, 1996. 181(2): p. 378-384.
Le, C.V., N.G. Ly, and M.G. Stevens, Measuring the contact angles of liquid
droplets on wool fibers and determining surface energy components. Textile
Research Journal, 1996. 66(6): p. 389-397.
Gu, Y.G. and D.Q. Li, Measurements of contact angles between an oil-water
interface and a fiber by the ACDPAC technique. Journal of Colloid and Interface
Science, 1998. 206(1): p. 288-296.
Gu, Y.G., D.Q. Li, and P. Cheng, A novel contact angle measurement technique
by analysis of capillary rise profile around a cylinder (ACRPAC). Colloids and
Surfaces a-Physicochemical and Engineering Aspects, 1997. 122(1-3): p. 135-149.
Wei, Q.F., et al., Dynamic wetting of fibers observed in an environmental
scanning electron microscope. Textile Research Journal, 2003. 73(6): p. 557-561.
Tao, W.Y. and B.J. Collier, The Environmental Scanning Electron-Microscope - a
New Tool for Textile Studies. Textile Chemist and Colorist, 1994. 26(2): p. 29-31.
Hartland, S., Surface and interfacial tension : measurement, theory, and
applications. 2004, New York ; Basel: Marcel Dekker. x, 619.
Rhee, H., R.A. Young, and A.M. Sarmadi, The Effect of Functional Finishes and
Laundering on Textile Materials .1. Surface Characteristics. Journal of the
Textile Institute, 1993. 84(3): p. 394-405.
Herb, C.A., J.L. Buckner, and J.R. Overton, The Effect of Cross-Sectional
Geometry on the Accuracy of the Fiber-Wetting Balance. Journal of Colloid and
Interface Science, 1983. 94(1): p. 14-24.
Sauer, B.B. and W.C. Kampert, Influence of viscosity on forced and spontaneous
spreading: Wilhelmy fiber studies including practical methods for rapid viscosity
measurement. Journal of Colloid and Interface Science, 1998. 199(1): p. 28-37.
Wagner, H.D., Spreading of Liquid Droplets on Cylindrical Surfaces - Accurate
Determination of Contact-Angle. Journal of Applied Physics, 1990. 67(3): p.
1352-1355.
Harnett, P.R. and P.N. Mehta, A Survey and Comparison of Laboratory Test
Methods for Measuring Wicking. Textile Research Journal, 1984. 54(7): p. 471478.
Rhee, H., R.A. Young, and A.M. Sarmadi, The Effect of Functional Finishes and
Laundering on Textile Materials .2. Characterization of Liquid Flow. Journal of
the Textile Institute, 1993. 84(3): p. 406-418.
Perwuelz, A., P. Mondon, and C. Caze, Experimental study of capillary flow in
yarns. Textile Research Journal, 2000. 70(4): p. 333-339.
Ferrero, F., Wettability measurements on plasma treated synthetic fabrics by
capillary rise method. Polymer Testing, 2003. 22(5): p. 571-578.
Volkov, V.A., B.V. Bulushev, and A.A. Ageev, Determination of the capillary
size and contact angle of fibers from the kinetics of liquid rise along the vertical
samples of fabrics and nonwoven materials. Colloid Journal, 2003. 65(4): p. 523525.
18
76.
77.
78.
79.
80.
81.
Ansari, N. and M.H. Kish, The wicking of water in yarn as measured by an
electrical resistance technique. Journal of the Textile Institute, 2000. 91(3): p.
410-419.
Ito, H. and Y. Muraoka, Water Transport Along Textile Fibers as Measured by an
Electrical Capacitance Technique. Textile Research Journal, 1993. 63(7): p. 414420.
Hoffmann, K.H. and M. Schreiber, Computational physics : selected methods,
simple exercises, serious applications. 1996, Berlin ; New York: Springer. xiv,
379.
van Remoortere, P., et al., Wetting behavior of a Lennard-Jones system. Journal
of Chemical Physics, 1999. 110(5): p. 2621-2628.
Manna, S.S., H.J. Herrmann, and D.P. Landau, A Stochastic Method to Determine
the Shape of a Drop on a Wall. Journal of Statistical Physics, 1992. 66(3-4): p.
1155-1163.
Lukkarinen, A., K. Kaski, and D.B. Abraham, Mechanisms of Fluid Spreading Ising Model Simulations. Physical Review E, 1995. 51(3): p. 2199-2202.
19
```